# A mathematical model of drying for hygroscopic porous media

Post on 06-Jun-2016

214 views

Embed Size (px)

TRANSCRIPT

A Mathematical Model of Drying for Hygroscopic Porous Media

A mathematical model is developed to simulate the drying of hygro- scopic porous media and, in particular, of wood. Drying rate experi- ments were performed using wood specimens and a nonhygroscopic porous ceramic solid and were simulated using the appropriate version of the drying model. Calculated model predictions are in very satisfac- tory agreement with experimental results. An examination of the relative impacts on drying of the transport mechanisms that comprise the model leads to meaningful interpretations of observed drying behavior. Con- trolling rate factors can be identified and different types of drying behavior specific to a given material or drying condition can be explained and understood through model simulation studies. Such capability can provide important guidance for drying process design and control.

M. A. Stanish, G. S. Schajer, Ferhan Kayihan

Weyerhaeuser Technology Center Tacoma, Washington 98477

SCOPE The drying of moist porous solids is a complicated

process involving simultaneous, coupled heat and mass transfer phenomena. Accordingly, drying behav- ior can be influenced by a rather large variety of inde- pendent factors, including, for example, ambient condi- tions of temperature, air velocity, and relative humidity, and solid properties such as density, permeability, and hygroscopicity. Extensive characterization of drying behavior using a strictly experimental approach consti- tutes a formidable challenge due to the excessively large number of variables that must be considered. The task becomes more manageable, however, with the help of a reliably realistic mathematical model of the drying phenomenon. Our objective is to develop such a tool to simulate drying behavior and therefore allow us to extend the results of experimental drying investiga- tions. In this way, the impact of the many variables on drying behavior can be examined and interpreted with- out having to resort to an extensive program of experi- mental testing.

The approach taken here represents advancement

Correspondence concerning this paper should bc addressed to Ferhan Kayihan. M. A. Stanish is with Energy International, Inc.. Bellevue. WA 98004.

of drying modeling and theory on several fronts. The mathematical description of the drying process is de- rived and maintained for the most general case; a com- prehensive set of fundamental heat- and mass-transfer mechanisms is coupled with thermodynamic phase equilibrium expressions in a way that accommodates either hygroscopic or nonhygroscopic materials. Heat transfer by both conduction and convection is included together with mass transfer by gaseous diffusion and bulk flow of gas and liquid through the void space and by bound-water diffusion through the solid matrix. Bound-water migration is expressed in terms of the dif- fusion of sorbed water driven by the gradient in the chemical potential of the bound molecules. While this concept of bound-water diffusion was previously sug- gested by Siau (1983) and others (Kawai et al., 1978), in this development a new, uniquely explicit expression for bound-water flux is derived in terms of temperature and vapor pressure gradients. Combination of all of these transport mechanisms in a single generalized model has provided the first opportunity to examine their individual roles, collective interactions, and rela- tive impacts on drying behavior.

AIChE Journal August 1986 Vol. 32, No. 8 1301

SIGNIFICANCE AND CONCLUSIONS A unique modeling approach based on fundamental

heat and mass transfer relationships and thermody- namic equilibrium provides a tool that is effective in predicting drying behavior and also useful in exploring and understanding the impact of important variables on the drying process. The inherently more complicated computational problem resulting from this approach was handled efficiently by developing a reduced but mathematically equivalent set of governing equations and numerically solving them using a specialized solver and an adaptive mesh scheme. Comparisons of model predictions with experimental drying data helped to verify the model for both hygroscopic and nonhygro- scopic drying.

Agreement between experimental results and model simulations was satisfactory; the model transport pa- rameters used were consistent and reasonable based on current knowledge of wood physical properties. Model profiles of temperature and moisture concentra-

tions were instrumental in interpreting observed drying rate behavior and identifying the rate-controlling pro- cesses.

With transport parameters derived from experimen- tal drying tests using the material of interest, the model can be used to simulate drying for a variety of condi- tions or material properties. In this way, a data base for drying behavior can be generated. Alternatively, sensi- tivity studies can be performed to determine the effect of different material properties on specific drying be- havior. In lumber processing, for example, given rea- sonable estimates for the range and distribution of wood properties represented within a lumber kiln charge, the corresponding distribution of expected dry- ing behavior can be predicted. In summary, the models simulation capabilities have significant implications in understanding drying behavior as well as in a range of application areas such as equipment design and pro- cess control.

Introduction Although substantial efforts have already been devoted to the

mathematical modeling of drying phenomena, the science re- mains far from perfected and therefore interest in the subject remains intense and widespread. Many of the previous ap- proaches have been limited to very specific applications with regard to either the material being dried or the particular drying regime or mechanism a t work. Extensive publications appear in the literature; however, a rigorous review is outside the scope of this paper. Compilations of recent developments appear in pub- lications edited by Ashworth (1982) and Mujumdar (1980, 1983). Applications to lumber drying have been surveyed by Rosen (1983).

In the following sections, a full description is given of the con- ceptual model and underlying assumptions on which the mathe- matical equations of the model are based. The full set of equa- tions is then presented, followed by a discussion of the methods employed for their numerical solution. Experimental drying test results using both hygroscopic and nonhygroscopic materials are then compared with model simulations in order to verify the model.

Model Development The drying phenomenon is viewed as a process of simulta-

neous mass and energy transfer occurring both inside and out- side the wood. Three moisture phases are recognized: free (liq- uid) water, bound water, and water vapor. Heat and mass trans- fer are coupled by the requirement that all phases remain in thermodynamic equilibrium a t the local temperature. Thus evaporation rates are determined locally by the balance between heat flows, temperature changes, and moisture flows, all subject

to phase equilibrium constraints. The overall drying phenome- non results from the simultaneous interaction of all of these pro- cesses.

The mechanisms of energy and mass transport are critical factors in such a conceptual description of drying. In this model, we try to identify all significant modes of transport and retain a quantitative mathematical expression for each. For example, an independent migration mechanism is postulated for each of the three moisture phases. Free water flows in bulk form driven by a gradient in the pressure within the liquid phase. Bound water migrates by a diffusion process that is driven by a gradient in the chemical potential of the sorbed water molecules. Water vapor and air are transported both by bulk flow driven by a gradient in total gas pressure and by binary diffusion driven by a gradient in the mole fraction of each component. Similarly, energy flows resulting from both conductive and convective mechanisms are included.

Modeling approach 1. Mass and energy transport are one-dimensional. 2. Gas, liquid, and solid are recognized as independent

phases with characteristic properties. Moisture can exist in any of the three different phases: a vapor in the gas, as free liquid, or as bound water within the porous solid matrix.

3. Local thermal and phase equilibria are always obeyed. If free liquid is present, the vapor and bound phases remain satu- rated a t the local temperature. In the absence of liquid, the bound water concentration and gas phase composition obey a sorption isotherm a t the local temperature.

4. Conditions at the two boundaries are completely indepen- dent of each other, may vary with time, and are characterized by convective transfer coefficients.

1302 August 1986 Vol. 32, No. 8 AIChE Journal

5. Migration of the bound water through the solid matrix occurs by a molecular diffusion process having a flux propor- tional to the gradient in the chemical potential of the bound mol- ecules.

6. Bulk convection of the liquid and gas phases follows Dar- cy's law. The effective permeability of the solid to both liquid and gas varies with the relative saturation of the void space within the solid.

7. Physical properties can vary with respect to both space and time. Transport properties that are dependent on changing physical properties therefore can also vary with respect to space and time.

Governing equations The model equations contain five dependent variables, con-

sisting of four mass densities and temperature. Densities are defined per unit volume of space in order to account for the por- osity of the solid matrix. For drying, the four densities are iden- tified as those of air, water vapor, bound water, and free water. The five dependent variables are described in terms of two inde- pendent variables, space and time. There are five governing equations: two mass balances (one each for air and for water), one energy balance, and two equilibrium equations (one de- scribing vapor-liquid saturation and a second for the bound water sorption relation).

Material and Energy Balances. In order to include mass transfer contributions from bulk flow, a mass balance on air must be satisfied. The conservation equation for air is:

where the effective local void fraction is t = td - ( p f / p w ) and the void fraction of dry solid is t,,.

In the absence of free water, the gas phase is assumed to be saturated with respect to the local bound water content and tem- perature. Bound water sortpion data for wood were correlated by Simpson (1971). We use the inverted form of his equation to explicitly relate vapor density to the bound water content and the temperature:

p u = ppt a4 + (a4I2 + - [ [ (5) where:

a, = -45.70 + 0.3216(T) - 5.012 x 10-4(T)2 (6) (7) a, = - 0.1722 + 4.732 x lO-,(T) - 5.553 x 10-6(T)2

a, = 1,417 - 9.430(T) + 1.853 x 10-'(T)' (8)

Boundary conditions Each of the three differential balance equations requires for

solution an initial condition and two boundary conditions. To satisfy the first requirement, initial profiles must be specified for temperature and for air and water densities:

a t t = 0:

T(z, 0) = T"(z ) (10) The conservation equation for water is:

By writing a balance equation for total water, we avoid having to specify explicitly the unknown rate of evaporation.

The energy balance is:

The rate of evaporation need not appear explicitly since convec- tive contributions from mass flow are included.

Phase Equilibrium Relations. If the local free water density is nonzero, the gas phase at that point is assumed saturated a t the local temperature. Saturated water vapor densities from steam tables were correlated over the range 300-500 K to within 1% accuracy. The saturated water vapor density within the solid is given by:

p Y 1 = (t) exp [-46.490 + 0.2179(T) - 5.0104 IO-~(T)Z + 3.4712 lo-' ( T ) ~ ] (4)

The initial moisture and temperature profiles must satisfy the local equilibrium constraints given by Eqs. 4 and 5.

The boundary condition requirements are satisfied by speci- fying three relations at each surface of the solid. First, the total gas pressure a t each surface must equal the ambient pressure:

a t z = 0:

at z = L:

where pressure is related to bulk density by p = R T p / M c Second, the total flux of moisture within the solid a t each sur-

face must equal the flux of water vapor through the external

AIChE Journal August 1986 Vol. 32, No. 8 1303

boundary layer:

a t z = 0:

n, + nb + nJ

In general, the convective mass transfer coefficients depend on the mass transfer rate itself; correlations derived from data for very low rates of mass transfer are corrected if mass fluxes become significant.

Third, the total energy flux within the solid a t each surface must equal the total energy flux through the external boundary layer:

a t z = 0:

aT noho + nuhu + nbht + nfhf - k -

aZ

at z = L:

aT noho + nvhu + nbht + nfhf - k - az

= M,Nuhu + M,N,h, + 4 ( t ) [ T ( L , t ) - T ; ( t ) ] (20) Heat transfer coefficients are also dependent upon the rate of mass transfer and are corrected if necessary.

Transport phenomena Mathematical relations for the flux terms in the governing

material and energy balance equations are derived from funda- mental equations for the appropriate transport mechanisms.

Liquid Phase. The migration rate of the free liquid phase is assumed to follow Darcy's law for flow through porous media. Therefore, the flux is proportional to the gradient in pressure within the liquid:

where the total pressure within the liquid phase is equal to the total local gas pressure less the capillary pressure, Pc, associated with the gas-liquid interface. Spolek and Plumb (1981) mea- sured capillary pressure in southern pine wood and suggested the following dependence on relative saturation (or fraction of void space occupied by liquid):

P, = 10,000(p,/tdpw)-0.6' (22)

The relative permeability of the solid to liquid flow is depen-

dent on the relative saturation and on the permeability of the solid when the voids are completely filled by liquid. Spolek and Plumb also reported that below a certain critical relative satura- tion, or irreducible saturation, the relative permeability fell to zero and liquid migration ceased due to a loss of continuity in the liquid phase. Above the irreducible saturation, the relative per- meability increases with increasing relative saturation, often in a sigmoid manner (Tesoro et al., 1974). Thus, for wood the effective permeability is expressed by:

where sir is the irreducible saturation. Gas Phase. The general expression of mass transport for the

flux of component a in a binary gas mixture relative to station- ary coordinates is:

With the convective or bulk-flow term expressed in the form of Darcy's law for flow through porous media, Eq. (24) gives the flux of...